Evaluation of microstructure and mechanical property ... investigated using X-ray diffraction,...
Embed Size (px)
Transcript of Evaluation of microstructure and mechanical property ... investigated using X-ray diffraction,...
Evaluation of microstructure and mechanical property variations in
AlxCoCrFeNi high entropy alloys produced by a high-throughput laser
Mu Li1, Jaume Gazquez2, Albina Borisevich3, Rohan Mishra1,4, and Katharine M. Flores1,4
1. Mechanical Engineering and Materials Science, Washington University in St. Louis, St.
Louis, MO 63130, USA
2. Institut de Cincia de Materials de Barcelona, Barcelona 08193, Spain
3. Materials Science and Technology Division, Oak Ridge National Laboratory, Oak Ridge,
TN 37831, USA
4. Institute of Materials Science and Engineering, Washington University in St. Louis, St.
Louis, MO 63130, USA
Twenty-one distinct AlxCoCrFeNi alloys were rapidly prepared by laser alloying an
equiatomic CoCrFeNi substrate with Al powder to create an alloy library ranging x = 0.15
1.32. Variations in crystal structure, microstructure and mechanical properties were
investigated using X-ray diffraction, scanning electron microscopy, scanning transmission
electron microscopy and nanoindentation. With increasing Al content, the crystal structure
transitioned from a disordered FCC to a mixture of disordered BCC and ordered B2 structures.
While the onset of BCC/B2 formation was consistent with previously reported cast alloys, the
FCC structure was observed at larger Al contents in the laser processed materials, resulting in
a wider two phase regime. The FCC phase was primarily confined to the BCC/B2 grain
boundaries at these high Al contents. The nanoindentation modulus and hardness of the FCC
phase increased with Al content, while the properties of the BCC/B2 structure were
insensitive to composition. The structure and mechanical properties of the laser-processed
alloys were surprisingly consistent with reported results for cast alloys, demonstrating the
feasibility of applying this high-throughput methodology to multicomponent alloy design.
Keywords: A. high-entropy alloys, B. phase stability, C. laser processing and cladding, D.
microstructure, F. nanoindentation
High entropy alloys (HEAs), also referred to as multi-principle element alloys, are of
growing interest as structural materials. HEAs are typically defined as random solid solutions
consisting of 5 or more metallic elements without a dominant solvent species . This
compositional complexity is often combined with a surprising simplicity in the crystal
structure, including disordered face centered cubic (FCC), body centered cubic (BCC), and
hexagonal close packed (HCP) structures . Although the formation of single-phase HEAs is
thought to result from the competition between the enthalpy of formation of intermetallic
compounds and entropy of mixing of the large number of components in the alloy, identifying
alloys which form these relatively simple structures within the vast multicomponent
composition space presents a significant challenge. To address this, in the present work we
apply a high-throughput laser deposition method  to efficiently create compositional
libraries in the AlxCoCrFeNi system. Compositional trends in microstructure and mechanical
behavior are then evaluated.
Among the most studied systems, Al-transition metal HEAs such as AlxCoCrFeNi and
AlxCoCrCuFeNi, have been found to have superior high-temperature strength as well as wear
and oxidation resistance . The unexpected properties beyond the capabilities of the
constituent elements can be attributed to the presence of multiple principal elements, which
are believed to induce in a range of complex effects, including lattice distortion and sluggish
diffusion [9,10]. AlxCoCrFeNi has been shown to transition from FCC to BCC with
increasing Al content , making it of particular interest for a study of microstructural
effects on properties.
Conventionally, to investigate phase formation and microstructure of complex metallic
alloys, researchers adopt a serial approach to prepare separate samples of each composition of
interest, typically via casting, melt spinning or powder metallurgy techniques. This requires
significant investment of time and resources. Laser-aided direct metal deposition provides a
way to produce extensive alloy libraries with much greater efficiency . The energy
provided by the laser creates a melt pool on the surface of a substrate, which can be a pure
substance or prealloyed. A metallic powder stream is then delivered to the melt pool to alloy
the material. By varying the powder composition and feed rate, a wide range of compositions
can be created on a single substrate. In this work, we apply this methodology to AlxCoCrFeNi.
Using the laser-processed alloy libraries, the evolution of the microstructure is characterized
by X-ray diffraction and electron microscopy, and mechanical properties are measured via
nanoindentation. The results are generally in good agreement with those obtained from a
serial casting approaches reported in the literature, while requiring significantly less time to
produce. This demonstrates the feasibility of applying the high-throughput methodology to
the design of complex crystalline alloys.
Materials and Methods
An equiatomic CoCrFeNi substrate was prepared using arc melting and casting. Raw
materials with purity greater than 99.9% were melted together in an argon atmosphere. The
resulting ingot was flipped and remelted at least 5 times on the water-cooled copper hearth to
improve homogeneity prior to casting into a copper mold to produce a 25 mm 25 mm 4.5
Compositional libraries were prepared using an Optomec MR-7 LENSTM system.
Twenty-five 2 mm 2 mm patches on the substrate surface were alloyed with varying
amounts of aluminum powder. The library had a total size of 14 mm 14 mm. In the Laser
Engineered Net Shaping (LENS) process, the laser creates a melt pool on the substrate surface,
into which a stream of the alloying powder is directed. The laser and powder stream raster
over the surface to create a layer; subsequent layers may be added to create a
three-dimensional deposit if desired. In the present experiments, the laser power and travel
speed during deposition were held constant at 150 W and 12.7 mm/s (30 in/min), respectively,
while the Al powder feed rate increased from 0.8 to 3.3 rpm in increments of 0.1 rpm for each
single-layer patch. Each patch consisted of 5 laser tracks with approximately 25% overlap.
The patches were remelted twice perpendicular to the deposition direction at a laser power of
200 W to improve mixing and compositional homogeneity of the alloyed region. The entire
deposition process to create the compositional library of 25 patches was completed in less
than 15 minutes. The surface of the library was then cleaned, ground, and polished for
The crystal structure of each patch was characterized via X-ray diffraction (XRD) with a
Rigaku D-MAX/A diffractometer with Cu-K radiation operating at 35 kV / 35 mA. Because
the spot size of the X-ray beam on the sample surface was larger than the 2 mm x 2 mm
square patches, a plexiglass mask with a tapered circular aperture (minimum diameter 2 mm)
was employed to block the signal from the surrounding material, enabling each patch to be
isolated for characterization. The diffraction signal from the mask was normalized and
subtracted from the XRD patterns.
The microstructures of the patches were characterized using a JEOL JSM-7001FLV field
emission scanning electron microscope (SEM) equipped with an Oxford HKL electron
backscattered diffraction (EBSD) detector. To most efficiently characterize the alloy library,
all of the SEM and related observations were performed in the plan view, i.e. perpendicular to
the substrate surface, rather than in cross section. The compositions of the patches were
measured using an Oxford INCA Energy 350 Si (Li) energy dispersive x-ray spectroscopy
system (EDS) on the SEM. For each sample, random points in 5 different grains were
In order to evaluate the effect of composition on mechanical properties, the hardness and
elastic modulus of each patch were measured using a Hysitron TI 950 Triboindenter equipped
with a diamond Berkovich indenter tip. Nanoindentation was performed on the polished plan
view surface at a loading and unloading rate of 600 N/s up to a maximum load of 3000 N.
Four indents were performed on each patch or, when possible, within each phase of interest,
with a spacing of at least 20 m between indents. Load-displacement data was continuously
captured and used to determine the modulus, E, and hardness, H, using the method described
by Oliver and Pharr  and assuming a constant value of Poissons Ratio of 0.25 for
Finally, detailed scanning transmission electron microscopy (STEM) was performed for a
selected composition using a Nion UltraSTEM 200 microscope, operating at 200 kV and
equipped with a fifth-order Nion aberration corrector and a cold-field emission gun. Due to
the destructive nature of STEM specimen preparation, an Al0.62CoCrFeNi specimen was
prepared separately from the main compositional library, using the same LENS parameters